Phase transitions and chromium(iii) luminescence in perovskite-type [C2H5NH3][Na0.5CrxAl0.5-x(HCOO)3] (x = 0, 0.025, 0.5), correlated with structural, dielectric and phonon properties.
Ptak, Maciej; Mączka, Mirosław; Gągor, Anna; Sieradzki, Adam; Bondzior, Bartosz; Dereń, Przemysław; Pawlus, S.; Physical chemistry chemical physics : PCCP 18 (2016) 29629–29640; doi:10.1039/c6cp05151k

data_7226710
_publ_section_title
;
 Phase transitions and chromium(iii) luminescence in perovskite-type
 [C2H5NH3][Na0.5CrxAl0.5-x(HCOO)3] (x = 0, 0.025, 0.5), correlated with
 structural, dielectric and phonon properties.
;
_journal_issue                   42
_journal_name_full               'Physical chemistry chemical physics : PCCP'
_journal_page_first              29629
_journal_page_last               29640
_journal_paper_doi               10.1039/c6cp05151k
_journal_volume                  18
_journal_year                    2016
_chemical_formula_sum            'C10 H22 Al N2 Na O12'
_chemical_formula_weight         412.26
_space_group_crystal_system      monoclinic
_space_group_IT_number           7
_space_group_name_Hall           'P -2yac'
_space_group_name_H-M_alt        'P 1 n 1'
_symmetry_space_group_name_Hall  'P -2yac'
_symmetry_space_group_name_H-M   'P 1 n 1'
_atom_sites_solution_hydrogens   geom
_audit_creation_method           SHELXL-2014/7
_audit_update_record
;
2016-07-22 deposited with the CCDC.
2016-10-03 downloaded from the CCDC.
;
_cell_angle_alpha                90
_cell_angle_beta                 90.966(3)
_cell_angle_gamma                90
_cell_formula_units_Z            2
_cell_length_a                   8.0343(3)
_cell_length_b                   9.2310(4)
_cell_length_c                   11.9465(5)
_cell_measurement_reflns_used    2167
_cell_measurement_temperature    270(2)
_cell_measurement_theta_max      26.4980
_cell_measurement_theta_min      2.7720
_cell_volume                     885.88(6)
_computing_cell_refinement       'CrysAlisPro 1.171.38.41 (Rigaku OD, 2015)'
_computing_data_collection       'CrysAlisPro 1.171.38.41 (Rigaku OD, 2015)'
_computing_data_reduction        'CrysAlisPro 1.171.38.41 (Rigaku OD, 2015)'
_computing_structure_refinement  'SHELXL-2014/7 (Sheldrick, 2014)'
_diffrn_ambient_environment      N~2~
_diffrn_ambient_temperature      270(2)
_diffrn_detector                 'CCD plate'
_diffrn_detector_area_resol_mean 10.6249
_diffrn_detector_type            Atlas
_diffrn_measured_fraction_theta_full 0.999
_diffrn_measured_fraction_theta_max 0.999
_diffrn_measurement_device       'four-circle diffractometer'
_diffrn_measurement_device_type  'Xcalibur, Atlas'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_probe          x-ray
_diffrn_radiation_type           'Mo K\a'
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0530
_diffrn_reflns_av_unetI/netI     0.0796
_diffrn_reflns_Laue_measured_fraction_full 0.999
_diffrn_reflns_Laue_measured_fraction_max 0.999
_diffrn_reflns_limit_h_max       9
_diffrn_reflns_limit_h_min       -9
_diffrn_reflns_limit_k_max       11
_diffrn_reflns_limit_k_min       -11
_diffrn_reflns_limit_l_max       14
_diffrn_reflns_limit_l_min       -12
_diffrn_reflns_number            6476
_diffrn_reflns_point_group_measured_fraction_full 1.000
_diffrn_reflns_point_group_measured_fraction_max 1.000
_diffrn_reflns_theta_full        25.668
_diffrn_reflns_theta_max         25.668
_diffrn_reflns_theta_min         2.789
_diffrn_source                   'fine-focus sealed X-ray tube'
_diffrn_source_type              'Enhance (Mo) X-ray Source'
_exptl_absorpt_coefficient_mu    0.204
_exptl_absorpt_correction_T_max  1.00000
_exptl_absorpt_correction_T_min  0.98297
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details
;
CrysAlisPro 1.171.38.41 (Rigaku Oxford Diffraction, 2015)
Empirical absorption correction using spherical harmonics,
 implemented in SCALE3 ABSPACK scaling algorithm.
;
_exptl_crystal_density_diffrn    1.546
_exptl_crystal_description       prism
_exptl_crystal_F_000             432
_exptl_crystal_size_max          0.21
_exptl_crystal_size_mid          0.18
_exptl_crystal_size_min          0.16
_refine_diff_density_max         0.224
_refine_diff_density_min         -0.317
_refine_diff_density_rms         0.056
_refine_ls_abs_structure_details
;
 Refined as an inversion twin.
;
_refine_ls_extinction_method     none
_refine_ls_goodness_of_fit_ref   1.039
_refine_ls_hydrogen_treatment    constr
_refine_ls_matrix_type           full
_refine_ls_number_parameters     240
_refine_ls_number_reflns         3186
_refine_ls_number_restraints     2
_refine_ls_restrained_S_all      1.038
_refine_ls_R_factor_all          0.0661
_refine_ls_R_factor_gt           0.0500
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'w=1/[\s^2^(Fo^2^)+(0.0350P)^2^] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0932
_refine_ls_wR_factor_ref         0.1047
_reflns_Friedel_coverage         0.994
_reflns_Friedel_fraction_full    1.000
_reflns_Friedel_fraction_max     1.000
_reflns_number_gt                2641
_reflns_number_total             3186
_reflns_threshold_expression     'I > 2\s(I)'
_cod_data_source_file            c6cp05151k2.cif
_cod_data_source_block           EtNaAl270K
_cod_depositor_comments
;
Adding full bibliography for 7226709--7226712.cif.

2023-11-23
Z value and formula fixed to values more according to usual
chemical conventions.                 miguel
;
_cod_original_formula_weight         206.13
_cod_original_formula_units_Z            4
_cod_original_formula_sum        'C5 H11 Al0.50 N Na0.50 O6'
_cod_database_code               7226710
_shelx_shelxl_version_number     2014/7
_oxdiff_exptl_absorpt_empirical_full_min 0.936
_oxdiff_exptl_absorpt_empirical_full_max 1.076
_oxdiff_exptl_absorpt_empirical_details
;
Empirical correction (ABSPACK) includes:
- Absorption correction using spherical harmonics
- Frame scaling
;
_shelx_res_checksum              16399